| ||Format||Pages||Price|| |
|6||$52.00||  ADD TO CART|
|Hardcopy (shipping and handling)||6||$52.00||  ADD TO CART|
Significance and Use
5.1 This method for investigating creep rupture of FRP bars is intended for use in laboratory tests in which the principal variable is the size or type of FRP bars, magnitude of applied force, and duration of force application. Unlike steel reinforcing bars or prestressing tendons subjected to significant sustained stress, creep rupture of FRP bars may take place below the static tensile strength. Therefore, the creep rupture strength is an important factor when determining acceptable stress levels in FRP bars used as reinforcement or tendons in concrete members designed to resist sustained loads. Creep rupture strength varies according to the type of FRP bars used.
5.2 This test method measures the creep rupture time of FRP bars under a given set of controlled environmental conditions and force ratios.
5.3 This test method is intended to determine the creep rupture data for material specifications, research and development, quality assurance, and structural design and analysis. The primary test result is the million-hour creep rupture capacity of the specimen.
5.4 Creep properties of reinforced, post-tensioned, or prestressed concrete structures are important to be considered in design. For FRP bars used as reinforcing bars or tendons, the creep rupture shall be measured according to the method given herein.
1.1 This test method outlines requirements for tensile creep rupture testing of fiber reinforced polymer matrix (FRP) composite bars commonly used as tensile elements in reinforced, prestressed, or post-tensioned concrete.
1.2 Data obtained from this test method are used in design of FRP reinforcements under sustained loading. The procedure for calculating the one-million hour creep-rupture capacity is provided in .
1.3 The values stated in either SI units or inch-pound units are to be regarded separately as standard. Within the text, the inch-pound units are shown in brackets. The values stated in each system are not exact equivalents; therefore, each system must be used independently of the other. Combining values from the two systems may result in nonconformance with the standard.
1.4 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.5 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
D883 Terminology Relating to Plastics
D3878 Terminology for Composite Materials
D5229/D5229M Test Method for Moisture Absorption Properties and Equilibrium Conditioning of Polymer Matrix Composite Materials
D7205/D7205M Test Method for Tensile Properties of Fiber Reinforced Polymer Matrix Composite Bars
E4 Practices for Force Verification of Testing Machines
E6 Terminology Relating to Methods of Mechanical Testing
E456 Terminology Relating to Quality and Statistics
E1012 Practice for Verification of Testing Frame and Specimen Alignment Under Tensile and Compressive Axial Force Application
ICS Number Code 91.100.40 (Products in fibre-reinforced cement)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM D7337 / D7337M-12(2019), Standard Test Method for Tensile Creep Rupture of Fiber Reinforced Polymer Matrix Composite Bars, ASTM International, West Conshohocken, PA, 2019, www.astm.orgBack to Top